Download (direct link):
4.1.3 Any optional chemical requirements from Table C-6, if desired,
4.1.4 Type of setting-time test required, Vicat or Gillmore. If not specified, the Vicar shall be used,
4.1.5 Any optional physical requirements from Table C-8, if desired.
NOTE 1—Attention is called to the fact that cements conforming to the requirements for all types may not be carried in stock in some areas. In advance of specifying the use of other than Type I cement, it should be determined whether the proposed type of cement is or can be made available.
5.1 The cement covered by this specification shall contain no addition except as follows:
5.1.1 Water or calcium sulfate, or both, may be added in amounts such that the limits shown in Table C-5 for sulfur trioxide and loss-on-ignition shall not be exceeded.
5.1.2 At the option of the manufacturer, processing additions may be used in the manufacture of the cement, provided such materials in the amounts used have been shown to meet the requirements of Specification C 465.
5.1.3 Air-entraining portland cement shall contain an interground addition conforming to the requirements of Specification C 226.
6. Chemical composition
6.1 Portland cement of each of the eight types shown in section 1 above shall conform to the respective standard chemical requirements prescribed in Table C-5. In addition, optional chemical requirements are shown in Table C-6.
7. Physical properties
7.1 Portland cement of each of the eight types shown in section 1 above shall conform to the respective standard physical requirements prescribed in Table C-7. In addition, optional physical requirements are shown in Table C-8.
8.1 When the purchaser desires that the cement be sampled and tested to verify compliance with this specification, sampling and testing should be performed in accordance with Practice C 183.
8.2 Practice C 183 is not designed for manufacturing quality control and is not required for manufacturer’s certification.
9. Test methods
9.1 Determine the applicable properties enumerated in this specification in accordance with the following test methods:
9.1.1 Air Content of Mortar—Test Method C 185.
9.1.2 Chemical Analysis—Test Methods C 114.
9.1.3 Strength—Test Method C 109.
9.1.4 False Set—Test Method C 451.
9.1.5 Fineness by Air Permeability—Test Method C 204.
9.1.6 Fineness by Turbidimeter—Test Method C 115.
9.1.7 Heat of Hydration—Test Method C 186.
Cement; Portland Cement C-25
TABLE C-5 Standard Chemical Requirements
Cement TypeA I and IA II and IIA III and IIIA IV V
Silicon dioxide (SiO2), min, % --- 20.0 --- --- ---
Aluminum oxide (Al2O3), max, % --- 6.0 --- --- ---
Ferric oxide (Fe2O3), max, % --- 6.0 --- 6.5 ---
Magnesium oxide (MgO), max, % 6.0 6.0 6.0 6.0 6.0
Sulfur trioxide (SO3),B max, %
When (C3A)C is 8% or less 3.0 3.0 3.5 2.3 2.3
When (C3A)C is more than 8% 3.5 D 4.5 D D
Loss on ignition, max, % 3.0 3.0 3.0 2.5 3.0
Insoluble residue, max, % 0.75 0.75 0.75 0.75 0.75
Tricalcium silicate (C3S)C max, % --- --- --- 35f ---
Dicalcium silicate (C2S)C min, % --- --- --- 40e ---
Tricalicum aluminate (C3A)C max, % --- 8 15 7e 5F
Tetracalcium aluminoferrite plus twice the tricalcium aluminateC --- --- --- --- 25f
(C4AF + 2(C3A)), or solid solution (C4AF + C2F), as applicable, max, %
A See Note 1 in section 4.
B There are cases where optimum SO3 (using Test Method C 553) for a particular cement is close to or in excess of the limit in this specification. In such cases where properties of a cement can be improved by exceeding the SO3 limits stated in this table, it is permissible to exceed the values in the table, provided it has been demonstrated by Test Method C 1038 that the cement with the increased SO3 will not develop expansion in water exceeding 0.020% at 14 days. When the manufacturer supplies cement under this provision, he shall, upon request, supply supporting data to the purchaser.